170 18 2MB
English Pages 83  Year 2022
The book covers the chronological development of synthetic approaches to make carbon nanotube mimics. It starts with the
170 74 5MB Read more
This Handbook covers the fundamentals of carbon nanotubes (CNT), their composites with different polymeric materials (bo
244 43 62MB Read more
Carbon nanotubes are exceptionally interesting from a fundamental research point of view. Many concepts of one-dimension
419 95 4MB Read more
Carbon nanotubes have been studied extensively in relation to fullerenes, and together with fullerenes have opened a new
483 55 7MB Read more
Carbon nanotubes have been studied extensively in relation to fullerenes, and together with fullerenes have opened a new
386 81 26MB Read more
This Handbook covers the fundamentals of carbon nanotubes (CNT), their composites with different polymeric materials (bo
199 79 69MB Read more
Raúl Hernández Sánchez, Saber Mirzaei, Edison A. Castro Portillo Carbon-Based Nanotubes
Also of Interest Nanomaterials. Volume : Electronic Properties Engg Kamakhya Prasad Ghatak, Madhuchhanda Mitra, ISBN ----, e-ISBN (PDF) ----, e-ISBN (EPUB) ---- Nanomaterials. Volume : Quantization and Entropy Engg Kamakhya Prasad Ghatak, Madhuchhanda Mitra, ISBN ----, e-ISBN (PDF) ----, e-ISBN (EPUB) ---- Environmental Functional Nanomaterials Qiang Wang, Ziyi Zhong (Eds.), ISBN ----, e-ISBN (PDF) ----, e-ISBN (EPUB) ----
Metallic Nanomaterials (Part A) S.S.R. Kumar Challa (Ed.), ISBN ----, e-ISBN (PDF) ----, e-ISBN (EPUB) ----
Raúl Hernández Sánchez, Saber Mirzaei, Edison A. Castro Portillo
Authors Dr. Raúl Hernández Sánchez Department of Chemistry University of Pittsburgh 219 Parkman Avenue Pittsburgh 15260 USA [email protected] Saber Mirzaei Department of Chemistry University of Pittsburgh 219 Parkman Avenue Pittsburgh 15260 USA [email protected] Dr. Edison A. Castro Portillo Department of Chemistry University of Pittsburgh 219 Parkman Avenue Pittsburgh 15260 USA [email protected]
ISBN 978-1-5015-1931-4 e-ISBN (PDF) 978-1-5015-1934-5 e-ISBN (EPUB) 978-1-5015-1253-7 Library of Congress Control Number: 2021950233 Bibliographic information published by the Deutsche Nationalbibliothek The Deutsche Nationalbibliothek lists this publication in the Deutsche Nationalbibliografie; detailed bibliographic data are available on the Internet at http://dnb.dnb.de. © 2022 Walter de Gruyter Inc., Boston/Berlin Cover image: Raúl Hernández Sánchez Typesetting: Integra Software Services Pvt. Ltd. Printing and binding: CPI books GmbH, Leck www.degruyter.com
Preface Scientists fascinate about bringing scientific challenges that seem impossible to the possible arena. Creating well-defined wire-like molecular tubes falls in this category. The writing of this book is inspired by recent synthetic developments toward this goal. In essence, the scientific community asks, how can molecular wires be reproducibly synthesized which provide reliable electronic properties that can be later translated into devices? Chapter 5 of this book presents what, in the authors’ opinion, are the first examples comprising the broadly defined area of atomically defined tubular conjugated nanotubes, an area that we expect will grow significantly in the years and decades to come. In chapter 1, we highlight the cornerstone discoveries around certain carbon allotropes to provide perspective on the evolving chemical techniques surrounding tubular contorted aromatics. This perspective is extended to the broad area of contorted aromatics and its beginnings in Chapter 2, providing a natural segue to the recently developed field of carbon nanorings in Chapter 3, and finally its extension to the most recently developed area of carbon nanobelts in Chapter 4. This book provides the reader with a concise and fundamental picture of the synthetic protocols developed to date to overcome the strain energy associated with bending aromatic surfaces, which is essentially the prerequisite to design conjugated nanotubes.
About the book
Carbon allotropes 1 1.1 Fullerenes 1 1.2 Cyclo[n]carbon 2 1.3 Carbon nanotubes 4 1.4 Graphene 6
Beginnings of radially contorted aromatics 2.1 Toward armchair geometries 9 2.2 Toward zigzag geometries 11
Carbon nanorings 17 3.1 [n]Cyclo-para-phenylenes 17 3.2 Polyaromatic-containing nanorings 20 3.3 Doped and mixed-aromatic nanorings 28
Carbon nanobelts 35 4.1 Armchair and chiral nanobelts 35 4.2 Zigzag nanobelts 38 4.3 Metal-containing nanobelt 40
Carbon-based nanotubes 43 5.1 End-cap-derived nanotubes 43 5.2 Tubularenes 45 5.3 Phenine nanotubes 48 5.4 Template-assisted porphyrin nanotubes
About the book Carbon, the chemical element, forms the atomic architecture of all forms of life. Many hypothetical carbon allotropes have been predicted, but only some are known, which can be divided into molecular and nonmolecular. Within the first family, we find fullerenes (being the most abundant C60 – buckminsterfullerene) and cyclic forms of carbon rings (e.g., cyclocarbon). The nonmolecular family is much larger and contains common materials like diamond, graphite, amorphous carbon, less common materials like lonsdaleite, and more recently discovered materials such as carbon nanotubes (CNTs) and graphene (a single carbon sheet within graphite). Although the discovery of CNTs has been contested, in the last two decades it has found widespread use as a composite material in batteries, coatings, supercapacitors, actuators, and lightweight electromagnetic shields . Advancing CNT synthesis toward the creation of nanotubes with monodisperse properties (e.g., diameter, chirality, and having a single wall) holds the promise to advance these prior applications and others where strict control of the CNT properties is required. Inspired by this synthetic challenge, scientists around the globe have embarked in developing bottom-up approaches to control the atomic definition of CNTs, and at the same time fine-tune the properties of the nascent nanotube. This book covers the development of bottom-up methodologies to prepare π-conjugated systems and the recent efforts to extend these systems along their main axis for the creation of radially and axially conjugated molecular nanotubes.
Author biographies Raúl Hernández Sánchez is an assistant professor in the Department of Chemistry at the University of Pittsburgh. He was born in Chihuahua, México. He obtained a B.Sc. from ITESM in Monterrey, México. Later, he received his Ph.D. in chemistry at Harvard University in 2015, where he investigated the coordination chemistry and electronic structure of iron clusters. In 2016, he moved to New York city as a Columbia Nano Initiative Postdoctoral Fellow exploring novel materials for nonaqueous redox flow batteries, and the synthesis and characterization of macromolecular contorted aromatics. In 2018, he started his research group working toward the development of supramolecular ligands for metal cluster development, nonspherical anion binding hosts, and the synthesis of tubular contorted aromatics, termed tubularenes. Saber Mirzaei received his M.Sc. in chemistry from Marquette University, where he worked on experimental and computational supramolecular chemistry, under the supervision of Prof. Rathore and Prof. Timerghazin. He joined Prof. Raúl Hernández Sánchez’s group at the University of Pittsburgh, carrying out Ph.D. studies to develop a new family of conjugated macrocyclic tubular arenes, termed tubularenes. Edison A. Castro Portillo was born in Nariño, Colombia. He obtained his B.Sc. from the Universidad de Nariño, Pasto, Colombia, in 2008; M.Sc. from the Universidad del Valle, Cali, Colombia, in 2011; and Ph.D. from the University of Texas at El Paso in 2017, under the supervision of Prof. Luis Echegoyen. He is currently a postdoctoral associate in the group of Prof. Raúl Hernández Sánchez at the University of Pittsburgh. His current research focuses on the design and synthesis of topologically unique organic compounds.
1 Carbon allotropes From an expensive natural diamond on your ring or watch, to an electronic component on your cellular phone or pacemaker, elemental carbon forms part of our daily lives in forms that often go unnoticed. Here we provide a summary of certain carbon allotropes that have attracted the attention of the scientific community. Based on their dimensionality, we first cover 0-D or molecular species fullerenes and cyclo[n]carbon, then 1-D carbon nanotubes (CNTs), and finally 2-D graphene. Chapter 1 provides context around the discovery of these allotropes and current state-of-the-art.
1.1 Fullerenes Fullerenes – a spheroidal allotrope of carbon composed of fused five- to seven-member rings – were detected for the first time during mass spectrometric studies of laserevaporated graphite in 1985 by Kroto and coworkers . However, the study of their properties, chemical reactivity, and applications was only possible after 1990, when Krätschmer and Huffman reported the synthesis of fullerene in macroscopic quantities . The highly symmetric icosahedral C60 carbon cage is composed of 12 pentagons and 20 hexagons (1.1, Figure 1.1), and owes its name to Richard Buckminster Fuller because of its similarity with the geodesic domes developed by the architect . Fullerene’s chemical reactivity is similar to that of an electron-deficient olefin , where additions usually take place at the 6,6 ring junctions. Additions to the 5,6 ring junctions ocurr only after rearrangement of the initial kinetic addition product to a 6,6 bond . Given their unique chemical properties, fullerene’s have impacted many fields within chemistry including; metal coordination complexes, drug delivery, spintronics, solar cells, catalysis, electronic devices and biological imaging [7–10]. Development of their chemical functionalization has been critically important to open up applications in these latter fields . In 1991, Smalley and coworkers reported the macroscopic synthesis of endohedral fullerenes (EFs), which are fullerenes that encapsulate metal atoms and small molecules in its interior. EFs are typically described as containing a positively charged guest, which is irreversibly, mechanically, and electrostatically trapped inside the negatively charged fullerene cage [12–15]. Since then, fullerenes were classified into two big groups: empty-cage fullerenes and EFs . In 1999, Dorn and coworkers reported the most abundant EF, Sc3N@Ih-C80 (1.2), and the third most abundant fullerene after C60 and C70 (Figure 1.1) . More recently, a new family of fullerenes called fullertubes was reported by Stevenson and coworkers in 2020 . Fullertubes are molecular single-wall CNT with half fullerene end-caps (e.g., C90 (1.3) in Figure 1.1). Contrary to
1 Carbon allotropes
CNTs, fullertubes can be prepared in a reproducible manner, exhibit a defined molecular weight, and are soluble in toluene and carbon disulfide.
Figure 1.1: Chemical structures of empty and endohedral fullerenes, and fullertubes.
Fullerenes resist high pressures; however, at pressures over 3,000 atmospheres they distort their shape, but upon pressure removal they return to their original structure . It has been theoretically calculated that a single C60 molecule has an effective bulk modulus of 668 GPa when compressed to 75% of its original size. This property establishes that fullerenes are harder than steel and diamond, whose bulk moduli are 160 and 442 GPa, respectively . Finally, fullerenes (C60 and C70) are electroactive and can be reversibly reduced with up to six electrons . This electron affinity is possible due to the presence of low-lying triply degenerate lowest unoccupied molecular orbitals .
1.2 Cyclo[n]carbon The newest allotropic form of carbon was reported in the middle of 2019. Similar to fullerenes and its analogues described in Section 1.1, this allotrope is also molecular in nature and is composed of a cyclic ring of n carbon atoms. At one extreme, it can be considered as an alternating form of bonding between single and triple covalent bonds (polyyne), and on the other as a cyclic cumulene. In fact, before the isolation and characterization of C60, R. Hoffmann proposed in 1966 a range of interesting nanorings composed solely of sp-hybridized carbon atoms, putting forward a novel idea of radially and perpendicularly oriented π-systems (Figure 1.2) . Over the next decade, extensive work was performed to synthesize the proposed cyclo[n]carbons. One general approach involved the use of masked alkyne macrocycles; for example, subjecting compound 1.4 to a gas-phase retro-Diels–Alder reaction under flash vacuum pyrolysis unveiled by mass spectrometry the formation of cyclo carbon, or C18. However, isolation of C18 proved challenging and its synthesis remained a target for decades to come [24–26].
Figure 1.2: Cartoon of a nanoring composed solely of carbon atoms with π-systems oriented in a (left) perpendicular and (middle) radial form as hypothesized by R. Hoffmann. Compound 1.4 was used as a precursor to cyclocarbon.
1 Carbon allotropes
Efforts on the synthesis and isolation of C18 (1.6) culminated in 2019 with its sequential preparation and isolation by Gawel, Gross, and Anderson . Their approach consists on the sequential elimination of carbon monoxide from C24O6 (1.5) on a bilayer of NaCl on Cu(111) at 5 K (Figure 1.3). Note that similar approaches had been explored before by Diederich et al. [24, 25, 28]. In one report, C18 was observed in the negative-ion laser desorption Fourier transform mass spectra of hexaketone 1.5. Alternatively, a stable hexacobalt complex (1.7) was synthesized as it consists of a masked cyclocarbon; however, the hypothesized oxidation of 1.7 as a method to unveil the masked C18 was not reported. Most importantly, experimental characterization of 1.6 in conjunction with theoretical modeling established that C18 is best described as a polyyne nanoring, in other words, a ring of carbon atoms bound to each other by alternating single and triple bonds [27, 29]. A year later, mid-2020, Gross and Anderson reported a follow-up on their work toward C18, whereby using a different synthetic approach increased their yield from 13% to 64% . In this case, they synthesized hexabromocyclocarbon 1.8 (C18Br6, Figure 1.3), which served as their new starting material, analogous to 1.5. The higher stability of 1.8 allowed them to thermally sublime it onto a NaCl/Cu(111) bilayer at 5 K without significant unmasking reactions. The experimental work on C18 laid the foundation for theoreticians to establish the correct bonding scheme within C18. In essence, the possibility of cumulenic rings was eliminated in favor of polyyne bonding with either D9h or C9h symmetry. It should be noted that the geometry of C18 has been studied extensively using different computational methods (e.g., density functional theory (DFT), Møller–Plesset, and quantum Monte Carlo) [30–34]. Surprisingly, the most applicable DFT functionals, like Becke-3Lee, Yang, and Parr (B3LYP) and the post-Hartree–Fock (HF) Møller-Plesset (MP2) method, indicated the cumulene ring as the ground state structure. Recently, Baryshnikov and Ågren reinvestigated the C18 structure using different DFT functionals and ab initio methods . Their results showed that the DFT methods are very sensitive to the amount of HF exchange (HFE) percentage, for example, B3LYP and PBE0 (PerdewBurke-Ernzerhof), with 20 and 25% HFE, respectively, cannot reproduce the correct geometry of C18. However, functionals with higher percentage of HFE like M06-2X (54% HFE) and BHandHLYP (Becke-half-and-half-LYP, 50% HFE) converged to a polyyne structure as the ground state, and the cumulene structure as a transition state at ~10 kcal/mol. Thermal energy at 5 K is much less than the calculated cumulenic transition state, supporting the ground state polyyne bonding observed by atomic force microscopy (AFM) at 5 K.
1.3 Carbon nanotubes CNTs are a 1-D carbon allotrope in the form of a cylinder, hence the tube designation, with a π-system orthogonal to the surface of the tube. The discovery of CNTs
1.3 Carbon nanotubes
Figure 1.3: Synthetic routes explored toward the synthesis of cyclocarbon, C18 (1.6).
1 Carbon allotropes
has widely been attributed to S. Iijima ; however, other sources point to earlier observations by Russian scientists L. V. Radushkevich and V. M. Lukyanovich in the early 1950s . Later, in 1960, R. Bacon  discovered carbon whiskers – a “rolled-up sheet of graphite layers” – while studying carbon grown in a dc arc at ~92 atmospheres of Ar and at 3,900 K. Bacon described these whiskers as being 1–5 µm in diameter, as highly flexible, with tensile strengths up to 2,000 kg/mm2, Young’s modulus >7 × 1012 dyn/cm2, and room temperature resistivity of ~65 ohm•cm. Years later, in 1976, Endo and coworkers  observed hollow carbon fibers prepared by benzene and hydrogen pyrolysis at ~1,100 °C with diameters of 20–500 Å and described them as the “annual ring structure of a tree.” Their catalytic process was patented in 1982. In 1991, in an attempt to discover the molecular structure of fullerenes and examine its crystal growth, Iijima observed a new material at the cathode side of the arc discharge reactor with a long and thin appearance . He named these materials “microtubules of graphitic carbon,” which were later addressed commonly as CNTs. Iijima acknowledged Bacon’s work on the formation of rolled-up single carbon-hexagonal sheet tubular filaments; however, Iijima did not observe overlapping edges in his filaments, instead he noticed concentric layers, and thus individual tubes with atomic size thickness. Two years later, Iijima  and Kiang  independently observed singlewalled carbon nanotubes (SWCNTs) and speculated that the nanotubes might be empty but under the right conditions the interiors may draw in species by capillary action. Also, to describe the helicity of these nanotubes it was suggested to follow Hamada’s notation , in which a CNT is represented by the indices (n, m), where n and m are the coefficients of unitary vectors v and u, respectively, as shown in Figure 1.4. Thus, three generic cases are recognized: first, when n = m the CNT is said to be “armchair”; second, when m = 0 (n, 0) the CNT is called “zigzag”; and third, when n ≠ m, the tube is called “chiral”. Also, when the difference n – m is a multiple of 3, the nanotube has metallic conductivity, while all others are semiconducting. Finally, even to this day, there is controversy as to who should be credited for the discovery of CNTs . CNT properties (thermal conductivity ~3,500 W/m•K , and semi- vs conducting electronic transport) have made them ideal materials for a range of applications, namely, composites for Li-ion batteries, flexible electronics, transparent conductors, sensors (optical, biological, and chemical), thermal interfaces, electronics (transistors, interconnects, and memory), membranes, and quantum wires . However, for applications requiring stricter control of the CNT properties and architectures, a tailored synthesis is still challenging and remains a current topic of intense research.
1.4 Graphene The IUPAC defines graphene as “a single carbon layer of the graphite structure, describing its nature by analogy to a polycyclic aromatic hydrocarbon of quasi-infinite size” (see gray background in Figure 1.4). Theoretical studies on graphene triggered
Figure 1.4: Representation of a carbon nanotube defined from a graphene fragment.
around 60 years ago [46–48]; however, its existence as a single sheet of carbon remained a hypothetical scientific curiosity for decades . Finally, in 2004, Novoselov et al. reported monocrystalline atom-thick graphitic films that were stable under ambient conditions . A year later, they reported their famous “scotch tape” method, which allowed everyone to obtain a few layer thin crystalline materials . These remarkable findings opened doors in almost all fields of science and awarded the Nobel Prize to Novoselov and Geim in 2010. This 2-D material is a zerogap semiconductor that exhibits exceptional electronic properties. When compared with SWCNTs, the electrical conductivity of graphene is ~60 times larger (64 mS/cm) . Interestingly, this value remains unchanged when tested at different temperatures. The large conductivity results from the very high electron mobility of graphene (200,000 cm2/V•s at room temperature), which is around 200 times higher than silicon . This very fast electron/charge mobility is directly correlated with the very high crystal quality (i.e., electrons can travel a long distance without significant scattering) .
1 Carbon allotropes
Another outstanding feature of graphene is its very high thermal conductivity, which has been investigated both experimentally and theoretically [54–56]. Thermal conductivity follows Fourier’s law (q = –kΔT), where q is heat flux, k is thermal conductivity, and ΔT is the temperature gradient. Molecular dynamic calculations showed thermal conductivity values around 1,500–3,000 W/m•K for SWCNTs, while the same study suggested higher values for graphene . However, experimental data on SWCNTs place their magnitude at ~3,500 W/m•K , while graphene’s thermal conductivity (single layer) has been measured to be 4,800–5,300 W/m•K . Finally, graphene’s properties have made this material an excellent choice to develop applications in detection, conversion, and emission of light, flexible graphene transistors, sensors, lithium–sulfur batteries, displays, structural composites, catalyst supports, polymer masterbatches, and functional inks, to name a few .
2 Beginnings of radially contorted aromatics Long before the discovery of carbon nanotubes (CNTs) [36, 43] and the synthesis of radially contorted [n]cyclo-para-phenylenes ([n]CPPs, discussed in Section 3.1), scientists attempted the bending of aromatic systems to create circular compounds displaying a radial orientation of their π-system. In this chapter, we provide a historical perspective prior to and around the time of the literature report by Iijima on “Helical Microtubules of Graphitic Carbon” in November 1991 , after which an exponential increase in research took place on this novel type of carbon allotrope that was shortly after described as CNTs. Below we divide the synthetic reports for radially contorted aromatics into those targeting armchair and zigzag geometries.
2.1 Toward armchair geometries Reports from Parekh and Guha in 1934 described the first attempts to create cyclic structures with their π-system oriented radially . It was hypothesized that under copper desulfurization conditions, compound 2.1 could provide the strained aromatic 2.3; however, it was concluded that complete desulfurization was not accomplished and instead the product obtained was 2.2 (Figure 2.1). Synthesis of cyclophane 2.1 was attempted decades later with no success. In 1976, Wong and Marvel showed that oxidation of 2.4 did not produce 2.1, as it was formerly believed, instead the oxidation reaction lead to trimeric (2.5) and/or tetrameric (2.6) compounds, in addition to a polymeric material [60, 61]. The prior unsuccessful syntheses were attributed to the large buildup of strain in the small radial aromatic compounds. To alleviate this hurdle, Vögtle and coworkers synthesized the larger sulfur-containing macrocycles 2.7 and 2.8, hoping that desulfurization conditions would provide the long-sought [n]CPPs (Figure 2.1) [62, 63]. Unfortunately, all macrocycle desulfurization attempts to synthesize [n]CPPs were unsuccessful. The alternative to desulfurization reactions included Diels-Alder transformations in pre-formed unsaturated macrocycles. A model reaction was provided by Miyahara et al., where macrocycle 2.9 in the presence of phenyl vinyl sulfoxide 2.10 provided cyclophane 2.11 in 15% yield (Figure 2.2) . Inspired by this precedent, Vögtle and coworkers embarked in the preparation of macrocycles 2.15 and 2.16 synthesized via Wittig cyclooligomerization of 2.12 and 2.14, or 2.13 and 2.14, respectively, which were explored as precursors in the formation of [n]CPPs. However, all attempts to synthesize CPP from 2.15, or CPP from 2.16, were unsuccessful. The Vögtle group pursued an additional alternative to radial aromatics. Their hypothesis was inspired by this notion: assuming aromatization could be carried out in the final step, it should be possible to establish the overall connectivity and later https://doi.org/10.1515/9781501519345-002
Figure 2.1: Desulfurization attempts in the synthesis of radial π-aromatics, [n]CPPs.
10 2 Beginnings of radially contorted aromatics
2.2 Toward zigzag geometries
induce aromatization of the strain-free macrocycle to produce the desired contorted ring structure. They synthesized macrocycles composed of aromatic rings and cyclohexane moieties. The purpose of the cyclohexane moiety was two-fold: first, it was thought that it would lend itself to establishing the curvature of macrocycles, and second, as a masked benzene ring assuming it could be aromatized in the last synthetic step, offsetting the strain induced from radially bending the conjugated aromatic. Toward this goal, 1,4-syn-diaryl molecules 2.17 and 2.18 were synthesized (Figure 2.3). The curvature observed in their crystal did not translate in the making of cyclic oligomers, and instead linear polymers were observed . To decrease the conformational fluxionality in solution, additional groups were added to the cyclohexane moiety resulting in the synthesis of 2.19; however, no cyclic oligomers were observed when inducing the aryl–aryl coupling reactions. To impart the desired rigidity, five- (2.20) and three-membered (2.21) rings were built into the bent diaryl precursor. However, para-halogenation was not reported for these compounds. Finally, in 1986, McMurray et al. published a report where diketone 2.22 (n = 1) was cyclized to cyclotetrakis(1,4-cyclohexylidene) (2.23, n = 1) using the reaction conditions that bear his name . Realizing the potential of this cyclative McMurray coupling, Vögtle’s group synthesized a longer diketone starting material , n = 2 (2.24), and subjected it to cyclization conditions obtaining macrocycle 2.25 (n = 2), which was expected to serve as a precursor for CPP. However, attempts following this strategy also proved unsuccessful.
2.2 Toward zigzag geometries The fundamental connectivity difference between the smallest radial benzenoid armchair versus zigzag CNT fragment is that the latter requires edge-fused aromatic rings, while the armchair geometry does not (e.g., [n]CPPs). Over the last 70 years, these radial benzenoid zigzag fragments have been called by different names such as cyclic polyacenes, [n]cyclacenes, superacenes, and belt[n]arenes. Here, structures like 2.26 are addressed as belt[n]arenes (Figure 2.5). These molecules were hypothetical targets first described by Heilbronner in 1954 (n = 12) . In the early 1880s, much research focused on the development of cyclophane chemistry. In this regard, Vögtle in his capacity as editor, and with ample experience targeting the synthesis of [n]CPPs, concluded the book series entitled Cyclophanes II in 1983 by proposing that “molecules looking like bracelettes, for example [beltarene], fully aromatic or partially aliphatic, belong to the stars under the phanes-to-be” . The first attempt to synthesize to belt[n]arenes was reported by Stoddart et al. in 1987 . Their hypothesis was that accessing cyclic structures of the type of 2.27 would provide access to “a fascinating new range of molecular architectures,” e.g., belt[n]arenes (2.26). Thus, employing consecutive Diels–Alder reactions on synthetically accessible bisdiene 2.28 and bisdienophile 2.29, they were able to obtain cyclic species 2.30,
Figure 2.2: Left: Precursor macrocycles tested in the synthesis of [n]CPP via Diels–Alder reaction. Right: Macrocycles synthesized via Wittig cyclooligomerization.
12 2 Beginnings of radially contorted aromatics
Figure 2.3: Curved diaryl precursors designed for the formation of cyclic oligomers as strain-free macrocycles prior the aromatization into [n]CPPs.
2.2 Toward zigzag geometries
2 Beginnings of radially contorted aromatics
Figure 2.4: Cyclo(1,4-cyclohexylidene) precursors explored in [n]CPP synthesis.
Figure 2.5: First synthetic attempts toward zigzag nanobelts, e.g., belt[n]arenes.
confirmed by solution 1H NMR studies and solid-state single-crystal X-ray diffraction data (SCXRD). Partial and full deoxygenation of 2.30 was achieved in a later publication . However, full aromatization to beltarene was not achieved [70, 71]. Synthesis of similar scaffolds ensued during the following years. A similar Diels–Alder strategy was employed by Schlüter et al. , where an AB-type monomer (2.32) was designed and synthesized in situ from 2.31. Compound 2.31 undergoes cyclobutene ring opening when refluxed in toluene (Figure 2.6). Polymerization initiates immediately upon formation of 2.32. Initial experiments showed a polymeric material and a low-molecular-weight species. This latter compound was isolated and crystallized, confirming the formation of a cyclic dimer (2.33). Increasing the dilution conditions to favor this cyclic dimer, Schlüter’s group was able to bring the yield to a remarkable 70% for 2.33. Aromatization of 2.33 into beltarene has not been reported. In 1996, Cory et al. reported the synthesis of macrocycle precursors for belt[n] arenes via double Diels–Alder cycloadditions. Macrocycle 2.36 is formed by slow simultaneous addition of flexible nonplanar bisdiene 2.34 and planar bisdienophile 2.35 in 1,4-dioxane under reflux . Spectral (NMR) and crystallographic (SCXRD) characterization confirmed the structure of 2.36. It is remarkable that the cyclic dimer is formed in 69% yield when chemical intuition would predict preference for a polymeric material. With 2.36 in hand, aromatization attempts seeking belt arene were pursued. Unexpectedly, treating 2.36 with pyridinium chlorochromate
2.2 Toward zigzag geometries
Figure 2.6: AB-type monomer approach reported by Schlüter et al. pursuing the formation of belt[n]arenes.
(PCC) under refluxing benzene produces anthraquinone derivative 2.37 . Hypothetically, 2.37 is the result of a double dehydrogenation of 2.36 producing an anthracene equivalent that is subsequently oxidized to anthraquinone. On a different approach, epoxidation of 2.36 followed by dehydrogenation with p-toluenesulfonic acid in refluxing benzene does not produce the expected anthracene, but instead bisdiene 2.38. Despite these efforts, formation of the fully unsaturated species, namely beltarene, were unsuccessful.
Figure 2.7: Double Diels–Alder cycloaddition reported by Cory et al., and dehydrogenation attempts toward belt[n]arene.
Above we described the historical development of synthetic attempts and strategies targeting macrocyclic aromatic systems. Even though all these efforts were unsuccessful, these investigations paved the way for future developments as described later in this book. This chapter described the main developments toward these conjugated nanorings from their early beginnings up to around the mid-1990s. Chapter 3 will present the accomplishments that finally opened the door to conjugated molecular nanorings and the more recent strategies reported in the literature.
3 Carbon nanorings The groundbreaking methodology to bend an aromatic system into a circular architecture was reported in 2008 by Jasti and Bertozzi . At its heart, the strain energy (SE) increases dramatically when a conjugated system bends radially, hence the question: is there a synthetic strategy that overcomes the challenge associated with bending the aromatic system away from planarity into a radial system? Similar to the approaches presented in Chapter 2, Jasti and Bertozzi’s methodology is based on first establishing the overall connectivity of the carbon nanoring, where the angular requirement is met by utilizing sp3 carbon atoms . The strainfree nanoring is then reductively aromatized providing [n]cyclo-para-phenylenes ([n]CPPs) – the shortest benzenoid radial segment forming an armchair carbon nanotube (CNT). In this chapter, we describe all of the fundamentally different methodologies reported to date and their molecular variability to synthesize [n]CPPs. Section 3.1 focuses exclusively on [n]CPPs. Next, Section 3.2 describes carbon nanorings formed by larger polyaromatic systems, and we conclude in Section 3.3 with mixed conjugated systems containing heteroatoms or other mixed-aromatic building blocks.
3.1 [n]Cyclo-para-phenylenes Circular molecules composed of benzene repeating units connected through their 1,4-positions are known in the literature as [n]cyclo-para-phenylenes . The first methodology to synthesize these species was reported in 2008 . It involved a masked aromatic ring in the form of a 3,6-syn-dimethoxy-cyclohexa-1,4-diene moiety (3.1 and 3.2) to provide the curvature needed to pre-form a macrocycle with negligible strain after Suzuki–Miyaura cross-coupling (Figure 3.1). Subsequent reductive aromatization of these macrocycles provided - (3.3), - (3.4), and CPP (3.5) in 43%, 52%, and 36% yield, respectively.
Figure 3.1: First [n]CPPs reported in the literature by Jasti et al. in 2008 .
3 Carbon nanorings
Shortly after in 2009, Itami and coworkers reported a similar approach, where instead of using a diene to curve the strain-free macrocycle they employed an embedded cyclohexane moiety as shown in compounds 3.6 and 3.7, which through stepwise Suzuki–Miyaura cross-coupling reactions with each other established the formation of macrocycle 3.8. This macrocycle was treated with stoichiometric amounts of p-TsOH in m-xylene at 150 °C for 30 min (microwave irradiation) providing CPP (3.9) in 62% isolated yield (Figure 3.2) . Note that aromatization of 3.8 was achieved through oxidative aromatization.
Figure 3.2: Selective synthesis reported in 2009 for CPP by Itami and coworkers .
A fundamentally different approach to [n]CPP was reported by Yamago et al. . They reasoned that cis-coordinated Pt-aryl complexes can be used as universal precursors to [n]CPPs. Since the cis-aryl substituents have a 90° angle between them, this Pt complex can serve as the corners of a strain-free square-shaped macrocycle. Following this hypothesis, the tetranuclear platinum macrocycle containing 4,4ʹ-biphenyl (3.11) was obtained by transmetalation of PtCl2(cod) with the organotin precursor 3.10 (Figure 3.3). Ligand exchange introducing 1,1ʹ-bis(diphenylphosphino)ferrocene provided compound 3.12, which undergoes bromine-induced reductive elimination  to afford CPP
Figure 3.3: First CPP reported in the literature.
(3.13) in 49% isolated yield. Similar to the previous [n]CPPs described in Figures 3.1 and 3.2, compound 3.13 displays fluorescence emission, its maximum λem is located at 540 nm. The three strategies described above established a fertile ground for vast research activity and inspired other chemists in the development of alternative methodologies giving access to functionalized [n]CPPs as described next. In 2014, Wang and coworkers reported a novel bent precursor 3.15, which was obtained from a Diels–Alder reaction between 3.14 and 1,4-benzoquinone. This dihydronaphthalene derivative (3.15) is the key intermediate in this synthetic protocol leading to the functionalized CPP (3.18) (Figure 3.4) . The following macrocyclic products were observed when 3.15 was subjected to a Ni-mediated homocoupling reaction: (a) syn and anti dimers (3.16) at 27% combined yield, and (b) the syn and anti trimers (3.17) at 11% combined yield. The dimeric species 3.16 did not yield the CPP derivative expected after aromatizing the macrocycle. In contrast, subjecting a mixture of both syn and anti trimers 3.17 to 2,3-dichloro-5,6-dicyano-1,4-benzoquinone (DDQ) at 70 °C for 2 days affords the CPP 3.18 species shown in Figure 3.4.
Figure 3.4: [n]CPP synthesis from a dimethoxynaphth-1,4-diyl unit.
3 Carbon nanorings
Also in 2014, Wegner et al. reported the first approach to [n]CPPs using a [Rh]catalyzed cycloaddition reaction to modify the strain-free macrocycle 3.19 prior to the oxidative aromatization step in air (Figure 3.5) . The result of this cycloaddition is the formation of a functionalized para-terphenyl moiety (3.20). Note that this approach is advantageous to introduce late-stage functionalization to the emerging [n] CPP (3.21). In fact, the side-group functionalization (R and R′ in Figure 3.5) introduced ring strains of around ±11 kcal/mol compared to the unsubstituted CPP ring SE of 72.2 kcal/mol . One year later, Tanaka et al. reported the synthesis of carboxylate-containing CPP, species 3.24. Similar to Wegner’s work, a functionalized para-terphenyl moiety (3.23) serves as the precursor for the reductive aromatization step that provides 3.24 in 33% yield (Figure 3.6a) . The triangle-shaped compound 3.23 is obtained through a [Rh]-mediated intermolecular cross-cyclotrimerization between 3.22 and di-tert-butyl acetylenedicarboxylate in 17% yield. As described by the authors, future work using this functionalized [n]CPPs will focus on solid-state applications by self-assembly. More recently, Tanaka’s research group developed an approach where a cyclic dodecayne (3.25) undergoes a four-fold [Rh]-catalyzed intramolecular cyclotrimerization to guide the synthesis of a functionalized CPP in 64% yield (species 3.26 in Figure 3.6b) . Most recently in 2020, Tsuchido et al. reported an interesting approach to CPP in a remarkable 59% overall yield. Their synthetic route starts by employing digold(I) complex 3.27, which in the presence of 4,4ʹ-diphenylene diboronic acid (3.28) forms a triangular hexagold(I) macrocycle (3.29) in 76% yield, where the corners are composed of digold(I) complexes as shown in Figure 3.7 . CPP is formed after the dinuclear gold centers are oxidatively chlorinated with PhICl2. Disproportionation of the putative Au(II)–Au(II) species forces aryl migration to form a chlorogold(I) complex and a neighboring chloro(diaryl)gold(III) center from which reductive elimination takes place to afford CPP in 76% yield (3.30) . Overall, these eight fundamentally different approaches provide a wide landscape of size variability. As a result [n]CPPs are known for n = 5–16 and 18 [77, 88–92], and also offer a significant toolbox for functionalized derivatives; some of which have been tested as luminescent solar concentrators , bioimaging tracers , ligands for metal coordination [95–97], various host–guest studies , and several other applications in supramolecular chemistry [91, 92].
3.2 Polyaromatic-containing nanorings Breaking the bottleneck to circularly bend aromatic systems paved the way for incorporating larger polyaromatic hydrocarbons (PAHs) into conjugated nanorings. In general, two research avenues have been explored: the first one consists in incorporating a single unit of PAH into a [n]CPP, whereas a second approach consists in forming the entire
Figure 3.5: Wegner’s [Rh]-catalyzed [2 + 2 + 2] cycloaddition followed by oxidative aromatization to synthesize CPPs.
3.2 Polyaromatic-containing nanorings
3 Carbon nanorings
Figure 3.6: Tanaka’s work on the synthesis of functionalized (a) CPP-based nanoring, which involves an intermolecular cyclotrimerization , and (b) CPP-based species formed through an intramolecular cyclotrimerization .
Figure 3.7: CPP (3.30) formation from reductive elimination of hexanuclear gold(I) complex.
3.2 Polyaromatic-containing nanorings
nanoring based solely on PAHs. In this chapter, we summarize PAHs that are used to construct nanorings while providing examples for each of these. Synthetic methods to incorporate naphthalene and anthracene into nanorings have been significantly developed, just behind those related to phenylene-based nanorings. Naphthalene can be incorporated into a nanoring through its [1,4] [99–102] and [2,6] [103– 105] positions. Figure 3.8 shows an example of the eight-membered 1,4-connected naphthalene nanoring (3.31) reported previously [101, 102]. Compound 3.31 was obtained through a [Pt]-mediated macrocyclization, akin to the strategy developed by Yamago et al. (Figure 3.3) . However, if naphthalene is linked into a nanoring through its [2,6] positions, it leads to chiral species, where for example a rotational barrier of 16 kcal/mol has been determined experimentally for cyclo-2,6-naphthylene . Anthracene has been incorporated as a single unit or several into nanorings, though a nanoring composed of anthracenyl units alone remains unknown. The different ways known in the literature to link anthracenyl within a [n]CPP: [1,4] , [2,6] , and [9,10] [108, 109]. Compound 3.32 is an example of an anthracenyl-embedded CPP . Similar to naphthalene, the 2,6-linked anthracenyl unit embedded within a nanoring provides chiral moieties; nonetheless, the two conformers interconvert readily by going through a density functional theory (DFT)-calculated rotational barrier of 8.6 kcal/mol . Phenanthrene, an isomer of anthracene, has been reported to form [3,9]-linked nanorings. Using the [Pt]-mediated macrocyclization route described in Figure 3.3, and starting with 3,9-borylated phenanthrene, Isobe et al. were able to obtain the compound cyclo-3,9-phenanthrenylene (3.33), which displays a complex case
Figure 3.8: Naphthalene, anthracene, and phenanthrene incorporated into nanorings. Red labels correspond to positions known in the literature to link these into nanorings, and in brackets are the linking positions when there is more than one way to link them. One nanoring example is shown for each PAHs.
3 Carbon nanorings
of cyclostereoisomerism . To quantify the isomerization barrier, the pure isolated enantiomers were subjected to variable temperature circular dichroism experiments, where the decay of the maximum CD signal at 419 nm was followed in the range 30–60 °C. An energy barrier of 25 kcal/mol was obtained from this analysis. Polyfluorenes are an attractive class of conjugated polymers with applications to organic electronics due to their high charge-carrier mobilities . Thus, with the advent of the synthetic strategies described in Section 3.1, macrocycles of fluorene became a target of great interest. Realization of 2,7-linked cyclicfluorenes (3.34) was possible through [Pt]-based chemistry, as described in Figure 3.3. Trimer and tetramer were synthesized in combined yields of 22% and 27% (Figure 3.9), respectively. Interestingly, rotamers of 3.34a were calculated to interconvert through a rotational barrier of 58.3 kcal/mol, much higher than those for 3.33, thus preventing interconversion even at 180 °C for 24 h . Not surprisingly, the DFT-calculated rotational barrier for 3.34b, which contains four fluorene units, decreases to 18.2 kcal/mol. Pyrene, a larger PAH relative to the previously discussed, has also been used in the formation of nanorings . Using pyrene as the only repeating unit to form nanorings was accomplished in 2014 when the four-membered pyrene-containing cycle, cyclo-2,7-pyrenylene (3.35, Figure 3.9), was reported in the literature . Structurally, 3.35 has the same circumference as CPP; however, the fused benzene rings in 3.35 makes it significantly more challenging to bend and thus its DFTcalculated SE is 93.7 kcal/mol, considerably higher than that of CPP at 72.2 kcal/ mol . Chrysene, similar to pyrene in that it has four fused benzene rings, has been linked into macrocycles through its [2,8] [115, 116] and [3,9]  positions giving rise to several atropisomers with remarkably persistent belt shapes (Figure 3.9). Of these, the 3,9-linked nanorings can be devised as fragments of zigzag nanotubes, which until 2012 were the last synthetic target of finite single-walled CNT models. The challenge was tackled when 3,9-borylated chrysene was subjected to Pt-mediated macrocyclization resulting in a single diastereomer with D4 point symmetry in 8% isolated yield (3.36) . Enantiomer interconversion was not observed even after 60 days at 200 °C. Antiaromatic PAHs have also been used to form nanorings. The first macrocycle of this kind incorporated the antiaromatic PAH dibenzo[a,e]pentalene (Figure 3.9). Following a similar synthetic strategy as that described in Figure 3.2, two units of 2,7-borylated dibenzo[a,e]pentalene were incorporated into a CPP (3.37) . Through nucleus-independent chemical shift calculations, it was determined that the bending of the dibenzo[a,e]pentalene units in the nanoring decreased its antiaromatic character. Alternative routes for inclusion of large PAH into nanorings include the in situ formation of PAH moieties within a preformed macrocycle. In this regard, dibenz[a, h]anthracene and dibenzo[c,m]pentaphene, linked through their [3,10] and [2,11]
Figure 3.9: Additional aromatic and antiaromatic PAHs incorporated into nanorings. Large acenes in 3.38 and 3.39 were formed in situ within a strain-free macrocycle.
3.2 Polyaromatic-containing nanorings
3 Carbon nanorings
positions, respectively, were formed through iterative ring closing metathesis from strain-free macrocycles containing pendant olefins. Subjecting those olefinic-containing cycles to Grubb’s second-generation catalyst, followed by reductive aromatization provided nanorings 3.38 and 3.39, as shown in Figure 3.9 . Compounds 3.38 and 3.39 can be viewed as π-extended systems relative to parent - and CPP, respectively. In both cases, the π-extended nanorings display a smaller calculated highest occupied molecular orbital (HOMO)–lowest occupied molecular orbital (LUMO) gap relative to their [n]CPP parents by ~0.1 eV. Within the larger PAHs used for nanoring formation, perylene, a common aromatic building block used in organic chemistry, has been reported to form chiral nanorings by linking it within a [n]CPP through its [3,9] positions (3.40, Figure 3.10) . Important to note, in contrast to [n]CPPs, the HOMO–LUMO transition in 3.40 is not symmetry forbidden. Attempts to use 3.40 to grow larger π-conjugated nanorings through Diels–Alder reactions only provided inconclusive results . Other large PAHs forming nanorings include the anthanthrene moiety, where literature reports confirm the synthesis of 2,8-anthanthrene-only  (3.41) and 4,10-anthanthrene-[n]CPP  nanoring systems. Interestingly, the rotational barrier of 3.41 is only 21 kcal/mol. Crystallographic determination of 3.41 indicates an average diameter of 14.1 Å. Dibenzo[g,p]chrysene, an extended PAH relative to chrysene shown before in Figure 3.9, has been reported to form a trimeric system linked through its [3,11] positions (3.42) . Using [Pt]-mediated macrocyclization of 3,11-diboryl dibenzo[g,p]chrysene provides almost exclusively the three-membered nanoring 3.42 in 23% yield. The atropisomers were separated in cholesterol-loaded silica gel, and their configuration assigned by comparison of their CD spectra with theoretical calculations. Importantly, these atropisomers do not interconvert in solution even after heating at 200 °C for 24 h. The first nanoring containing five-membered rings was reported in 2017 by Isobe and coworkers by subjecting 5,15-diborylated rubicene to platinum-mediated macrocyclization conditions . The trimer (3.43a) and tetramer (3.43b) products were formed in 0.2% and 1.4% yields, respectively. Note however that those yields comprise several stereoisomers (e.g., 3.43b has four stereoisomers). These rubicene-containing nanorings have absorption tails that extend up to 640–670 nm, which are significantly shifted considering rubicene by itself has onset of absorption at 530 nm, indicating an extension of the π-system in the nanoring relative to monomeric rubicene. Interestingly, 3.43 are not fluorescent, a feature attributed to the presence of pentagons in the nanoring structure. Last, the largest PAHs forming part of a nanoring are tribenzo[b,n,pqr]perylene  and hexa-peri-hexabenzocoronene (Figure 3.10) [125–131]. The first one features a type of molecular crown (3.44) comprising a CPP-like substructure, which absorbs light between 260 and 460 nm with λmax at 325 and 356 nm, and emits at λem = 459 and 488 nm with a quantum yield of 12.7%. DFT calculations provide a SE of ~80 kcal/mol for 3.44. Also, this species can accommodate and host
Figure 3.10: Largest PAHs incorporated into nanorings.
3.2 Polyaromatic-containing nanorings
3 Carbon nanorings
C60 with a binding constant (Ka) of 3.34 × 106 M−1 in toluene. Finally, the cyclic tetramer formed by linking 2,11-hexa-peri-hexabenzocoronene (3.45) has a larger diameter than 3.44 since it contains a CPP-like substructure; thus, the SE of 3.45 at 49 kcal/mol correlates with the expectation of being lower relative to that of 3.44. Importantly, the bigger size of 3.45 allows it to host C70, as determined from fluorescence quenching experiments, with a Ka of 1.07 × 106 M−1 in toluene.
3.3 Doped and mixed-aromatic nanorings Incorporation of heteroatoms into aromatic systems is devised as a method of altering its electronic structure, which is also as an intrinsic doping method. However, synthetic protocols to achieve this doping in molecular nanorings, as those described above, are scarce and limited. Despite much efforts in the last decade, this is a long-standing challenge for the design and creation of novel materials [132, 133]. Perhaps the most common method to incorporate heteroatoms (e.g., N, O, and S) into cyclic or acyclic aromatic systems is by starting with precursors already containing these atoms, as in a number of well-known heterocycles. Ultimately, the resulting heteroatom-containing nanorings display tuned absorption and emission properties, coordination chemistry, and redox potential. The first doped nanoring was reported in 2012 by Itami and coworkers. This is an CPP-like nanoring containing two 2,2ʹ-bipyridyl units linked into the nanoring through their [4,4ʹ] positions (3.46, Figure 3.11) . Nanoring 3.46 is halochromic, meaning that its optical properties change based on pH. Specifically, when 3.46 is in the neutral state it displays blue fluorescence, and when protonated its emission is red-shifted becoming green fluorescent. The same 2,2ʹ-bipyridyl moiety was later introduced into a smaller nanoring, this time as part of the backbone of an CPP. Most importantly, the newly reported synthetic protocol allows a more general approach toward incorporating the 2,2ʹ-bipyridyl unit into other nanorings . With compound 3.47, Jasti et al. demonstrated the metal coordination ability of the 2,2ʹ-bipyridyl moiety when forming part of a strained nanoring. To this effect, Pd(II)- and Ru(II)-nanoring coordination compounds showed that upon excitation of the metal complex, the excited state resides primarily in the nanoring portion. Other aza-containing nanorings have been reported including one, two, and three nitrogen atoms incorporated into the structure of an CPP (3.48–3.50) [135, 136], or CPP . The general idea behind these modifications is to study the optoelectronic properties of these family of nanorings at different levels of nitrogen doping. In addition, methylation to form a pyridinium equivalent represents a post-synthetic modification to further tune the nanoring’s properties. Following this strategy, it was demonstrated that the HOMO and LUMO levels can be tuned independently opening the door for future applications of these nanorings as organic electronic materials.
3.3 Doped and mixed-aromatic nanorings
Figure 3.11: Nitrogen-containing nanorings.
Diazapyrenylene is an alternative building block for nitrogen doping. Employing a platinum-mediated macrocyclization, nanorings containing a skeleton of [n] CPP, with n = 12 (3.51a), 16 (3.51b), and 20 (3.51c), were synthesized in yields of 4%, 11%, and 3%, respectively . Crystallographic data of 3.51b indicates its diameter to be 21.3 Å. Other nitrogen-containing building blocks used for nanoring synthesis include N-functionalized carbazoles connected through their [2,7] positions (3.52) [139, 140]. From the easily available calixcarbazole macrocycle [141, 142], Lu and Chen were able to derivatize the calix macrocycle and rigidify it through a Yamamoto cross-coupling forming compound 3.53 . This species displays green fluorescence and a quantum yield of 0.39. Interestingly, two well-defined electrochemical oxidation events are observed via cyclic voltammetry of 3.53 with onset potential
3 Carbon nanorings
(Eoxonset) at 0.17 and 0.43 V versus Fc/Fc+. In contrast, reduction of 3.53 only displays ill-defined events with Eredonset of −1.85 V versus Fc/Fc+. From this data, a narrow electrochemical HOMO–LUMO gap of 2.02 eV is obtained. The rigidity of 3.53 is best exemplified by its DFT-calculated electronic structure which indicates a fully delocalized HOMO and LUMO. Donor–acceptor nanoring systems have been developed by modifications of the synthetic strategies described in Section 3.1. In this regard, tetracyanoanthraquinodimethane connected at its [2,6] positions with a CPP forms a nanoring (3.54) with a remarkably low LUMO level at −3.55 eV versus vacuum, which also displays a 1.93 eV HOMO–LUMO gap . This type of curved donor–acceptor system provides new molecular designs for organic electronic material applications. Sulfur-doped nanorings are rare; however, in 2015 Itami et al. reported a series of nanorings that can be devised as the mixture of [n]cyclothiophene and [n]CPP to form [n]cyclophenylenethienylene (CPT), which have the architecture displayed by 3.55 (Figure 3.12), marking the first of its kind alternating 1,4-phenylene and 2,5thienylene nanorings . The final step yield to make nanorings 3.55a, 3.55b, and 3.55c, are 13%, 24%, and 3%, respectively. As in [n]CPPs, DFT calculations indicate that the HOMO–LUMO transition is symmetry-forbidden. In contrast to [n]CPPs, as the [n]CPT ring size increases, the HOMO–LUMO gap decreases, which is mainly attributed to an energy lowering of the LUMO levels, while the energy of the HOMO level remains practically unchanged. Related sulfur-containing nanorings were synthesized through the protocol described in Figure 3.4 . In this regard, compound 3.15 was further derivatized following three more synthetic steps to effectively replace the bromide atom functionality with a 2-iodothiophene moiety, producing the key precursor for nanorings 3.56a (dimer) and 3.56b (tetramer). These two nanorings were investigated by electrochemical methods finding that 3.56a displays a reversible and irreversible oxidation centered at +0.41 and +0.79 V versus Fc/Fc+, respectively. Similarly, 3.56b displays three reversible oxidation processes occurring at +0.53, +0.84, and +0.98 V versus Fc/Fc+. Contortion of the final nanoring by sulfur incorporation was produced by cyclizing 3,7-dibenzo[b,d]thiophene, and its S,S-dioxide, into tetrameric products (3.57, Figure 3.12) . Interestingly, 3.57a and 3.57b display similar absorption and emission bands relative to its CPP parent. In contrast, the electrochemical properties of these nanorings are markedly different from those of CPP. Reductively, 3.57a and 3.57b display a single reduction event at −2.07 and −1.57 V versus Fc/Fc+ (CPP’s reduction is at −2.33 V), respectively. Oxidatively, 3.57a displays well-separated stepwise oxidation events at +0.74 and +0.96 V versus Fc/Fc+ ( CPP’s oxidation occurs at +0.59 V), while 3.57b shows no oxidative activity up to +1.5 V versus Fc/Fc+. Benzothiadiazole (BT) has been used to tune the optoelectronic properties of nanorings as an S,N-doping building block. Two recent approaches report on this
3.3 Doped and mixed-aromatic nanorings
Figure 3.12: Sulfur-containing nanorings.
strategy: the first one by Jasti et al. incorporates a single BT unit into a CPP (3.58) , whereas the work of Tan and coworkers  report a CPP containing four evenly spaced BT units (3.59). Aside from a weak low energy absorption band in 3.58 that extends past 500 nm, the absorption envelope and λmax of  CPP and 3.58 are rather similar. In contrast, 3.58 has a remarkable Stokes shift of 237 nm (λem = 571 nm) compared to 128 nm observed in CPP (λem = 466 nm). In comparison, the Stokes shift in CPP is 90 nm (λem = 428 nm) , and this shift increases mildly to 142 nm (λem = 569 nm) in 3.59. Finally, there is a vast landscape of other molecular radially conjugated architectures involving nonconventional PAHs, Möbius strips, unusual connectivity, or those that fall outside of the definitions outlined in this chapter so far. Rigidifying the nanoring by limiting the degrees of freedom of phenylene rotation is a strategy adopted to maintain the radial disposition of the π-system. For instance, a nanoring similar to 3.24, however, with a smaller CPP backbone reported by Wang et al.
3 Carbon nanorings
 was used as precursors in the formation of 3.60 (Figure 3.13) . This nanoring (3.60) is composed of three indeno[2,1-a]fluorene-11,12-dione-2,9-diyl units, which are formed in situ by transforming dimethyl phthalate moieties through a stepwise combination of (1) trifluoroacetic acid and trifluoroacetic acid anhydride at 75 °C, followed by treating the resulting mixture with (2) Eaton’s reagent (7.7 wt% P2O5 in methanesulfonic acid) at 75 °C. DFT calculations show that the anti-isomer (3.60) is more stable (ΔG°) than the syn-isomer (all carbonyls pointing in the same direction) by 4.3 kcal/mol, and the barrier separating anti to syn isomers (ΔG‡) is 23.3 kcal/mol. Overall, this strategy reduces the number of rotatable bonds to just three single C–C bonds. The first hydrocarbon catenane – a mechanically interlocked molecule – was reported in 1983 by Schill et al. . It was composed of sp3 carbon atoms. However, until recently creating a similar catenane based on sp2 carbons was an unmet challenge. In 2017, Müllen and coworkers were the first to report on the existence of all-benzene catenanes (interlocked [n]CPPs), and trefoil knots by ion mobility mass spectrometry . In trying to achieve a controlled synthesis for sp2 carbon-based catenanes, Fan et al. hypothesized that incorporation of phenanthroline into the nanoring would facilitate the interlocking of two nanorings by making use of metal coordination. Thus, in 2018 they published a manuscript where coordination of Cu(I) by two phenanthroline moieties served as a template to grow the radial nanoring, which also helped to maintain the ring interlocking. As a result, the topology they obtained resembles that of a Möbius strip (3.61 in Figure 3.13) . Related work toward the synthesis of Möbius nanorings was reported by Tanaka et al. using a similar strategy as that described in Figure 3.6b, whereby increasing the size of 3.25 and employing a chiral phosphine supporting ligand, (S)-BINAP, they were able to induce intramolecular cyclotrimerizations forming a Möbius-shaped functionalized CPP . Synthesis and isolation of interlocked [n]CPPs were reported shortly after by Segawa et al. . In research published in July 2019, they describe the first examples of allbenzene catenanes, CPP-interlocked-CPP (3.62) and CPP-interlocked-CPP, and a trefoil knot molecule composed of 24 p-phenylenes (3.63). This challenging synthesis was accomplished through a spirobi(dibenzosilole) intermediate, which mimics the function of the metal complex [(phen)2Cu(I)] described above in Fan’s work, and also has the advantage of quantitative desilylation by treatment with fluoride ion in ethanol , thus liberating a biphenyl equivalent that forms part of the interlocked [n] CPP. Interestingly, the fluorescence emission spectrum of CPP-interlocked-CPP is almost identical to pure CPP, and nothing like that of CPP, indicating that upon excitation fast energy transfer to CPP is the leading mechanism of relaxation to ground state . Later on, through a similar approach, Segawa and coworkers described the synthesis of CPP-interlocked-CPP . Additional methods to restrict the orientation of the π-system employ sterically demanding fragments. In this regard, the cone-shaped compound 3.64 is rigid and
3.3 Doped and mixed-aromatic nanorings
Figure 3.13: Other radially conjugated aromatic nanorings.
unable to rotate forming a segment of a (6,6)CNT . Unrelated to the synthetic protocols described so far, Itami and coworkers developed a three-step synthesis to 3.65 from ethyl pillararene, which already has the built-in property of being a strain-free macrocycle. Nanoring 3.65 can be considered as a methylene-bridged 
3 Carbon nanorings
CPP . DFT calculations indicate that 3.65 has a SE of 110.2 kcal/mol, larger than CPP at 96 kcal/mol, and furthermore a smaller HOMO–LUMO gap relative to CPP. Aside from phenylene-based nanorings, there is a large class of porphyrin-based nanorings that Anderson and others have reported in the literature . Perhaps the most extensive family of these compounds is the template-assisted formation of porphyrin nanorings pioneered by Anderson and coworkers . In general, a template such as T6 coordinates a Zn-porphyrin molecule at each of the pyridinic ends, positioning the six Zn-porphyrins in a circular array proximal to each other and at the right distance to undergo oxidative coupling under Pd/Cu catalysis, using iodine as an oxidant, to form a cyclic system as shown in nanoring 3.66 (Figure 3.13) . Structurally, species like 3.66 can be regarded as formed by alternating [5,15]-linked porphyrins and butadiynes. Note that if the template is removed from the nanoring species, the porphyrin units tend to have low rotational barriers [164, 165], similar to large [n]CPPs. Another version of porphyrin nanorings was reported by Osuka and coworkers in 2015. These compounds comprise [2,12]-linked Ni-porphyrins forming tri, tetra, and pentameric cyclic species . Interestingly, the trimeric cyclic Niporphyrin features a HOMO–LUMO gap of 2.07 eV, which is smaller than the monomeric Ni-porphyrin at 2.28 eV. Finally, the field of conjugated molecular nanorings has grown considerably, especially in the last dozen years when [n]CPPs were finally obtained and characterized. This field will likely grow and mature, translating the properties of these nanorings into material applications and beyond.
4 Carbon nanobelts Although radial belt-like architectures were the target of synthesis since early in the past century, structures defined as “a closed loop of fully fused edge-sharing benzene rings” were only realized for the first time in 2017 . Since the number of published articles on these types of compounds is relatively small, every report will be described in this chapter and the advances they provide to this growing family of compounds.
4.1 Armchair and chiral nanobelts The first type of nanobelt described in the literature was reported by Gleiter et al. in 2008 . It features a [6.8]3cyclacene (4.1), which consists of annulated six- and eight-membered rings (Figure 4.1). Note that 4.1 does not resemble a fragment of a CNT. Single crystal data indicates that conjugation between the double bond and the aromatic rings is minimal, given the average dihedral angle of 71.9° between the plane of the benzene rings and the plane of the double bond. Nanobelt 4.1 displays λmax at 220 nm, shoulders at 278 and 290 nm, and emits at λem = 370 nm. Related N-containing nanobelts were reported by Wu et al. in 2021. They obtained compounds 4.2a–4.2d employing bis(o-aminobenzophenone) through a self-condensation reaction (Figure 4.1) . Optically, compounds 4.2a through 4.2d display a monotonic increase in λmax from 265, 277, 292, and 295 nm, respectively. While 4.2a and 4.2b do not absorb light above ~420 nm, 4.2c and 4.2d have absorption bands extending until around 500 nm. Nanobelt 4.3 was reported in early 2017 , which resembles 4.1 and 4.2 in that it has a large dihedral angle between benzene rings of around 51.2–82.2°, and between double bond and benzene rings in the range 72.6–74.5°. Similar to 4.1, compound 4.3 does not resemble a CNT fragment. Nanobelt 4.3 was designed following a similar protocol to buckycatcher . It has a lowest energy absorption band centered at 236 nm and displays an emission band at 340 nm. It has a DFTcalculated strain energy of 20.8 kcal/mol. In 2020, Wang and coworker reported that resorcin[n]arenes  – a well-known family of macrocyclic arenes – could be derivatized into truncated cone structures resembling 4.1. Nanobelt 4.4 was synthesized in three steps from resorcin[n]arene, n = 4 or 6 . This approach benefits from having the macrocycle preformed prior to establishing the radial π-system. Overall, the double bond connecting the benzene units is introduced by derivatizing the OH groups in the starting resorcin [n]arene to vinyl moieties, which are treated with Grubbs-II catalyst to form the final product. Nanobelt 4.4 displays host–guest properties by encapsulating small solvent molecules (e.g., MeCN and MeNO2). https://doi.org/10.1515/9781501519345-004
4 Carbon nanobelts
After a long history of attempts at the synthesis of CNT belt fragments , Itami and coworkers were finally able to provide a synthetic route to achieve this monumental task. The realization was accomplished in 2017 by sequential Wittig reactions and intramolecular Yamamoto couplings. This strategy resulted in 4.5, albeit in a reaction yield of around 1% (Figure 4.1) . Compound 4.5 resembles a segment of (6,6)CNT and is a structural isomer of the elusive cyclophenacene. Nanobelt 4.5 has a diameter 0.2 Å larger than that of CPP at ~8.1 Å . Since 4.5 is more rigid and has less degrees of freedom than CPP, its DFT-calculated strain energy is 23 kcal/mol higher than that of CPP at 96 kcal/mol [83, 176].
Figure 4.1: Gleiter’s (4.1) , Wu’s (4.2) , Miao’s (4.3) , Wang’s (4.4), and Itami’s (4.5)  molecular nanobelts. Ar = Ph, (4-t-Bu)C6H4 or (4-n-Bu)C6H4.
DFT calculations performed on 4.5 demonstrate that its frontier molecular orbitals are distributed over the whole nanobelt. This nanobelt has a lowest energy absorption band centered at 400 nm and a weakly absorbing window extending up to ~500 nm.
4.1 Armchair and chiral nanobelts
Note that 4.5 fluoresces at λem = 635 nm, in contrast to the nonfluorescent CPP. Subsequent publications by Itami et al. report analogues of 4.3 containing 16 and 24 fused benzene rings . Important to note: while in [n]CPPs λmax is ring sizeindependent (all absorbing at ~350 nm), the absorption of 4.5 and its larger analogues have absorption bands that red-shift with increasing size. Interestingly, emission of 4.5 and its larger analogues displays a monotonic blue-shift as the size increases. Finally, although counterintuitive, DFT calculations show that the HOMO–LUMO gap in these nanobelts becomes larger as the ring size increases, similar to what happens in [n]CPPs .
Figure 4.2: Miao’s armchair (4.6) and chiral (4.7) nanobelts as fragments of (12,12) and (18,12)CNT, respectively. Aromatic framework (red/orange rings) of Tilley’s axially extended nanobelt 4.8.
In 2019, Miao and coworkers designed two nanorings: the first is a functionalized CPP, while the second is a nanoring composed of six alternating units of 2,6-naphthalene with six functionalized 1,4-phenylenes, blue and green backbones shown in Figure 4.2, respectively, which they used to derivatize into large armchair nanobelt 4.6 and chiral nanobelt 4.7 (Figure 4.2) . Nanobelts 4.6 and 4.7 resemble a short segment of (12,12) and (18,12)CNT, respectively. Their radial π-surface is the largest reported in a nanobelt as of summer 2021. These
4 Carbon nanobelts
nanobelts were synthesized by π-expansion through Scholl reactions on their precursors (radial backbone highlighted in blue and green in Figure 4.2). Cyclization of the precursor nanorings produced changes in SEs of 45.8 to 54.2 kcal/ mol when forming 4.6, and 39.1 to 28.2 kcal/mol for the synthesis of 4.7. While the general notion is an increase in SE after cyclization, as in 4.6, the observed decrease toward 4.7 demonstrates that certain belt-forming reactions may actually relieve strain. In fact, the higher-than-expected yield of 66% for 4.7 is attributed to this strain relieving transformation. The optical properties of the precursors to 4.6 and 4.7 are almost identical having λmax and λem of 310 and 450 nm. All the absorption bands of 4.6 and 4.7 are red-shifted relative to their precursors. For instance, 4.6 has a lowest absorption band centered at 466 nm, while for 4.7 it is at 427 nm with a shoulder at 447 nm. Regarding emission, fluorescence bands appear at 498 and 532 nm for 4.6, while for 4.7 these bands are located at 464 and 492 nm. Visually, solutions of 4.6 and 4.7 appear green and blue, respectively. Finally, electrochemical HOMO levels were measured at −5.69 and −6.04 eV for 4.6 and 4.7, respectively. Recently, Tilley et al. reported a nanobelt that can be regarded as a fused diagonal cross-sectional fragment of a (6,6)CNT. For better visualization, the aromatic framework of this compound, 4.8, is inscribed into a (6,6)CNT as shown in Figure 4.2. The construction of 4.8 involves an initial ring fusion, followed by macrocyclization and diversification through a Diels–Alder reaction, finishing with a final ring fusion via a Yamamoto coupling in an overall yield of 26% . The identity of this compound was confirmed via 1H NMR, where 1H resonances indicated the expected C2h symmetry, in addition to single-crystal X-ray diffraction determination, from which an end-to-end length of 15.6 Å was established for the aromatic core. The optical properties of 4.8 revealed an absorption onset located at 486 nm and optical HOMO–LUMO gap of 2.7 eV, similar to the measured electrochemical HOMO–LUMO gap of 2.9 eV. Nanobelt 4.6 displays a sharp emission maximum at 491 nm, which decays monotonically until 600 nm.
4.2 Zigzag nanobelts Nanobelts with a zigzag-CNT geometry, historically called [n]cyclacenes and more recently belt[n]arenes [66, 68, 168, 181–183], have been more challenging to synthesize. DFT calculations indicate that one possible reason for this synthetic challenge is that these types of belts have a small band gap, and that triplet ground states are observed when the ring size reaches nine or more fused benzene rings . Thus, zigzag nanobelts are expected to be reactive given their electronic nature resulting from their inherent strain energy . Despite these challenges, the first nanobelt with this geometry was reported by Wang and coworkers in 2020, when they observed an in situ
Figure 4.3: Zigzag nanobelt 4.9 and 4.10 reported almost simultaneously by Itami, Segawa, and coworkers, and Chi et al., respectively. Miao’s nanobelt 4.11 is constructed via Scholl reactions.
4.2 Zigzag nanobelts
4 Carbon nanobelts
formation of a functionalized beltarene under MALDI-TOF conditions . However, isolation of this compound was not reported. Soon after Wang’s publication, two research groups, Segawa, Itami, and coworkers [185, 186], and at the same time Chi et al. , independently reported the synthesis and characterization of functionalized beltarene (4.9) and beltarene (4.10) as shown in Figure 4.3, respectively. Single-crystal X-ray diffraction data confirms that 4.9 represents a fragment of zigzag (18,0)CNT, while 4.10 represents that of (12,0)CNT. DFT-calculated strain energies are reported to be 63.3 kcal/mol for 4.9ʹ (R = H), while for 4.10ʹ (R = H) the authors report 186.5 and 72.9 kcal/mol based on two different hypothetical homodesmotic reactions. Nanobelt 4.9 features a broad absorption band with λmax at 336 nm and a weak lowest energy absorption peak at 405 nm. Regarding emission, compound 4.9 fluoresces at 407 and 432 nm with a shoulder at 457 nm upon excitation with UV light. This data provides an optical band gap of ~3 eV. Nanobelt 4.9 has an average diameter of 14.05 Å; in comparison, the smaller nanobelt 4.10 features a 9.2 Å diameter. The optical properties of 4.10 display a broad absorption band at 332 nm with an additional weak band at lower energy (405 nm), similar to 4.9. The fluorescence of 4.10 is red-shifted in comparison to 4.9, with major emission peaks at 422 and 442 nm. These two closely related belt[n]arenes, 4.9 and 4.10, are the first compounds of a large family of zigzag CNT fragments that hold the promise to unveil unprecedented properties and reactivity. Most recently, Miao et al. expanded on their previous approach toward armchair 4.6 and chiral 4.7 nanobelts, to generate zigzag nanobelts. The key feature comprises the incorporation of meta-phenylene units, which besides alleviating the strain in the precursor nanoring, it masks the zigzag-forming site of the eventual nanobelt. The aromatic framework of the nanobelt reported by Miao et al., 4.11 , is shown by the red and orange rings inscribed in the (16,0)CNT fragment shown in Figure 4.3. The aromatic region of its 1H NMR confirms its molecular C2h symmetry. Given its size, it displays affinity for C60 forming a 1:1 adduct with a binding constant (Ka) of (6.6 ± 1.1) × 106 M−1, as determined from fluorescence quenching. The DFTcalculated SE of 4.11ʹ (R = H instead of n-Pr) is 67.5 kcal/mol, which is smaller than beltarene calculated at 82.8 kcal/mol . Compound 4.11 displays broad absorption below 480 nm with a λmax at ~350 nm and a weak low absorption band at ~435 nm, likely due to the HOMO-to-LUMO transition. This same compound exhibits photoluminescence with two major peaks at 446 and 477 nm. This strategy put forward by Miao et al., using Scholl reactions and strategically positioned metaphenylene units, presents a viable route to expand on zigzag nanobelts.
4.3 Metal-containing nanobelt Belt-shaped compounds with radial aromaticity are not limited to carbon-only compounds. To this end, Yamada and coworkers reported a strained porphyrinic system
4.3 Metal-containing nanobelt
that is unable to rotate like those described in Section 3.3. This metal-containing nanobelt, 4.12, is shown in Figure 4.4.
Figure 4.4: Yamada’s nickel-containing porphyrinic nanobelt.
Nanobelt 4.12, which can be regarded as a porphyrin trimer, is synthesized in one step from (i) 1,2,4,5-tetra(pyrrol-2-ly)benzene, 4-(t-butyl)benzaldehyde, and BF3•OEt2 for 12 h, followed by (ii) oxidation with DDQ, and (iii) metalation with Ni(OAc)2•4H2O in 4% yield. Crystallographic data corroborates its C3h ideal symmetry, where the Ni–Ni distances are on average 8 Å. Optically, 4.12 displays λmax at 512 nm, while the monomeric Ni–porphyrin shows λmax at 537 nm, indicative of minimal electronic interaction between the metalated porphyrins within 4.12. Electrochemical measurements confirm that this nanobelt is able to accept and deliver up to five electrons with first oxidation and reduction potentials observed at +0.31 and −1.70 V versus Fc/Fc+, respectively. Finally, UV–vis titration experiments with C 60 display a binding stoichiometry in which two C 60 molecules sandwich 4.12. Note that the molecular structure of 4.12 displays two concave surfaces, which are attributed as the sites for C60 binding. As described by the authors, future work includes tuning of the electronic structure of this type of nanobelt through incorporation of other transition metals and examination of the properties of the larger porphyrinic belt analogues.
5 Carbon-based nanotubes Decades of research has shown that axially extending a radial π-conjugated surface, similar to forming a tube, remains a current challenge. Tubular species able to delocalize electrons, akin to a wire, are exceedingly rare . The chemistry to “stack” nanobelts along their rotational axis in order to form radially and axially conjugated tubular species remains very much under research and development. This chapter provides an analysis of the few conjugated molecular nanotubes (CMTs) reported to date. The molecular nanotubes described here are reported in the scientific literature and share the following characteristics: (1) their π-surface is radially and axially delocalized; and (2) are conformationally restricted or locked, which means that covalent bonding allows them to maintain a tubular shape preventing any possibility of rotational wall movement, which is achieved by a built-in end-cap in some of the nanotubes described herein. Hence, nanorings of (poly)aromatic building blocks, as described in Section 3.2, are not considered here as carbon-based nanotubes. Also, in contrast to carbon nanobelts (described in Chapter 4), the carbon-based nanotubes described here do not need to contain fused benzene rings. In this chapter, we describe several compounds that fulfill these criteria and highlight any relevant synthetic details that made the realization of these possible.
5.1 End-cap-derived nanotubes Short molecular nanotubes have been synthesized from strain-free precursors that bring the reacting partners close in space. This approach was followed by Stępień et al. whose team reported in 2015 the synthesis of two highly strained nonclassical nanotubes from tricarbazole-based precursors . The larger of the two compounds is shown in Figure 5.1 as synthesized when tricarbazole species 5.1 is subjected to Yamamoto coupling conditions to form nanotube 5.2 in 7% yield. Formation of 5.2 inherently produces a small internal opening on one end and is closed on the other end by a benzene fragment. DFT-calculated SE of 5.2 is 144 kcal/mol. It displays an onset of an irreversible ill-defined electrochemical oxidation at ca. +120 mV vs Fc/Fc+. Optically, 5.2 displays a broad absorption with λmax at 319 nm and a long absorption tail extending until around 550 nm, forming a yellow solution when 5.2 is dissolved in dichloromethane. This nanotube emits strongly at two maxima, 440 and 465 nm, with an extended emission tail displaying a weak band at ~630 nm and decaying to zero around 700 nm. Nanotube 5.2 has a fluorescence quantum yield of 6%. Mechanistically, the formation of 5.2 begins with oxidative additions of Ni(bpy)(cod) to the aryl halides to form a triangular trinickel macrocycle, which has been calculated to be highly exothermic with an energy gain exceeding 200 kcal/mol in the gas phase. Sequential reductive https://doi.org/10.1515/9781501519345-005
5 Carbon-based nanotubes
elimination (RE) steps, forming biaryl covalent linkages, increase strain by about 30–40 kcal/mol per step.
Figure 5.1: Synthesis of end-cap-derived nanotubes 5.2 and 5.4.
A similar in size end-cap-derived nanotube was reported by Scott and coworkers in 2012 using the functionalized corannulene 5.3 as a precursor to 5.4, described by the formula C50H10 (Figure 5.1) . The authors comment that although “the synthesis of 5.4 required years to develop, [. . .] ultimately [it was] accomplished in just three steps from corannulene.” The synthesis developed by Scott et al. involves treating 5.3 at high temperature under vacuum. These forcing conditions are similar to early reports on CNT synthesis, where arc discharge methods were common, reaching >1,700 °C, which were later substituted for chemical vapor deposition at milder temperatures (2 g, 70% yield). The octabromo derivative 5.9 maintains a tubular structure when small alcohols are present in solution creating a belt of hydrogen bonds around the benzimidazole fragments. Suzuki–Miyaura cross-coupling reaction of 5.9 with 1,3-phenylboronic acid bis(pinacol) ester affords tubularene 5.10 in a 3.3% isolated yield (Figure 5.3) . Similar reaction conditions with 2,7naphthalenediboronic acid bis(pinacol) ester provides 5.11 in 2.5% yield. 1H NMR spectra of 5.10 and 5.11 reflect their C4-symmetric structure. Their DFT-optimized structures display diameters of ~9.5 and ~12.7 Å for 5.10 and 5.11, respectively, indicating that the synthetic strategy developed for tubularenes is not only able to modulate the overall geometry of the target tubularene but also allows for tuning of the tube’s diameter. The SEs of 5.10 and 5.11 are 42.2 and 61.9 kcal/mol, respectively, which are counterintuitive since 5.11 has a larger diameter than 5.10 . However, bending of the top rim fused arenes (naphthalene units) of 5.11, which can be regarded as partial belt[n]arenes as described in Section 4.2, appears to add significant strain into the overall system. Tubularenes 5.10 and 5.11 display an almost identical absorption envelope above 300 nm with λmax at 305, 318 and 335 nm, where the onset of absorption occurs around 350–360 nm. Fluorescence spectra for these tubularenes display emission bands at λem = 364 and 376 nm for 5.10, whereas those for 5.11 are located at λem = 365 and 405 nm. Red-shifting of the low-energy emission band for 5.11 is likely related to its larger radial π-surface. The Stokes shift for 5.10 and 5.11 is almost the same at around 2,460 cm−1, and about a third of the Stokes shifts observed for tubularenes 5.7 and 5.8. Note that others have reported on the synthesis of zigzag nanotubes templated by calix[n]arenes, similar to 5.10; however, none of the optoelectronic properties were published . The synthetic approach toward tubularene species may open the door to a large family of novel contorted aromatic compounds highly modular in length, diameter, porosity, and optoelectronic properties, which will extend the toolbox of novel organic electronic materials.
5.3 Phenine nanotubes Synthesizing CMTs is a challenging task, and even more difficult is the incorporation of defects at well-defined locations within the nanotube architecture. To address this challenge, Isobe and coworkers created a methodology to build cylindrical species containing tens of benzene (phenine) units covalently joined together through their 1, 3, and 5 positions. These nanotubes are built from strain-free floppy macrocycles, which are
5.3 Phenine nanotubes
functionalized in their top and bottom peripheries with functional groups that allow the zipping up of the macrocycle into a nanotube.
Figure 5.4: Isobe and coworkers’ synthesis of strain-free macrocyclic precursors 5.15.
The first members of these so-called strain-free macrocycles were synthesized from m-terphenyl species 5.12a (Figure 5.4). Compound 5.12a was homocoupled by subjecting it to Yamamoto cross-coupling conditions with Ni(cod)2 to produce the functionalized cyclo-meta-phenylene (CMP) compound 5.13a in 84% yield . This CMP unit was devised as the repeating unit in a hypothetical macrocycle formed by connecting 5.13a through the R2 position. To accomplish this feat, Bpin groups were installed in the R2 position by exposing 5.13a to Ir-catalyzed borylation
5 Carbon-based nanotubes
producing 5.14a in 92% yield. This building block was used in conjunction with Yamago’s Pt-macrocyclization conditions (Figure 3.3) to afford strain-free trimer (n = 3, 9%), tetramer (n = 4, 25%), and pentamer (n = 5, 11%) macrocycles 5.15a as shown in Figure 5.4. Notice that as n goes from 3 to 5, the floppiness of the macrocycle increases. A later report expanded on the physical characterization of macrocycles of the form of 5.15a . A small feature, yet fundamentally important, was observed in the smallest trimeric congener, where it was noticed that it displayed a broad red-shifted absorption. This shoulder is ascribed to extended radial π-conjugation resulting from the more rigid macrocycle with n = 3. Also, important to mention is that the tetrameric species with a diameter of 1.65 nm binds C70 with an association constant (Ka) of 4.7 × 104 M−1 (toluene-d8), similar to the reported Ka of 1.5 × 105 M−1 , and 5.3 × 105 M−1 for C70 in CPP (diameter = 1.51 nm, toluene-d8) . The strain-free macrocycles 5.15a were rigidified by introducing alternative functionality at R1. Thus, the trimethylsilane (TMS) group was removed by iododesilylation with ICl. These polyiodinated macrocycles (R1 = I) were placed under Suzuki–Miyaura cross-coupling reaction conditions with 3-t-butyl-5-chlorophenylboronic acid pinacol ester to provide the axially extended macrocycles 5.16a in